# Anisotropy of the ΔE Effect in Ni-Based Magnetoelectric Cantilevers: A Finite Element Method Analysis

^{1}

^{®}), Technische Universität Ilmenau, Postfach 100565, 98684 Ilmenau, Germany

^{2}

^{®}), Technische Universität Ilmenau, Postfach 100565, 98684 Ilmenau, Germany

^{*}

## Abstract

**:**

^{−1}for (110) in-plane-oriented Nickel at a magnetic bias flux of 1.78 mT. The results achieved by FEM simulations are compared to the results calculated by the Euler–Bernoulli theory.

## 1. Introduction

## 2. Model Details

#### 2.1. Analytic Description of the ΔE Effect in Nickel

#### 2.2. Description of the Finite Element Model

#### 2.3. Limits of the Proposed Model

## 3. Results

#### 3.1. Magnetostriction and Bending

#### 3.2. Eigenfrequency Behavior in the Magnetic Field

^{−1}which is comparable to other references based on soft magnetic FeGa or FeCo compounds. Sensors based on FeCoSiB are able to reach higher sensitivities by a factor of 5–10 in combination with a high degree of optimization. The theoretical results still remain significantly higher but are similar between soft magnetic FeCoSiB and the (110)-oriented Nickel. The given simulated FeCoSiB sensitivity of 48 T

^{−1}is obtained for the second bending mode, which yields a higher value than the first/natural mode. The first bending mode should yield a sensitivity approximately 20% lower according to the data in [11], leading to an almost identical result as Ni(110). The direct growth of (110) in-plane-oriented Nickel is experimentally difficult on a hexagonal substrate such as AlN. However, there are approaches using 150 nm thick Au/Ge interfacial layers [10] for larger sensors. Additional interface engineering is needed to see whether this configuration can be scaled down to MEMS structures. Further similarities between FeCoSiB and Nickel apply to the saturation magnetostriction [45] or the density [46] leading to a similar mass inertness in the vibrational behavior, e.g., in passive operation. However, MEMS structures are less suitable for passive operation due to the size dependence of the limit of detection [47]. In actively operated sensors, the limit of detection plays a negligible role, which is why the sensitivity in combination with the dynamic range are the figures of merit to be used.

## 4. Conclusions

^{−1}at a magnetic bias flux of 1.78 mT. Such a high sensitivity is nearly identical to that of frequently used soft magnetic materials, such as FeCoSiB. However, the comparison between simulations and experiment was limited due to some assumption of the simulation that were in the general case not true in real sensor samples and partly not easy to achieve even if they would lead to an improved sensitivity. Especially, the magnetostrictive film is normally not single crystalline and it is more realistic to generate a polycrystalline microstructure with a strong preferential orientation. Other limitations, as listed in Section 2.3, were the 2D instead of 3D modeling, which changed the shape anisotropy behavior, and also of course no defects such as point defects or dislocation were considered, which would change the magnetization behavior. In any case, the simulation results gave a good indication of a high potential for further optimizations of the sensor performance, regardless of the used material.

## Author Contributions

## Funding

## Institutional Review Board Statement

## Informed Consent Statement

## Data Availability Statement

## Conflicts of Interest

## Appendix A

**Table A1.**Fit constants for the magnetostriction and magnetization curves according to Equation (A1).

Parameter | ${\mathsf{\kappa}}_{\mathit{hkl},\mathit{sat},1}$ | ${\mathsf{\kappa}}_{\mathit{hkl},\mathit{sat},2}$ | ${\mathsf{\alpha}}_{1}$ (${10}^{-4}$ m/A) | ${\mathsf{\alpha}}_{2}$ (${10}^{-4}$ m/A) | ${\mathit{H}}_{0,1}$ (A/m) | ${\mathit{H}}_{0,2}$ (A/m) |
---|---|---|---|---|---|---|

${\lambda}_{100}$ | −1.61$\phantom{\rule{0.166667em}{0ex}}\xb7\phantom{\rule{0.166667em}{0ex}}{10}^{-5}$ | −1.34$\phantom{\rule{0.166667em}{0ex}}\xb7\phantom{\rule{0.166667em}{0ex}}{10}^{-4}$ | 2.17 | 1.40 | 0 | −22,132 |

${\lambda}_{110}$ | −7.95$\phantom{\rule{0.166667em}{0ex}}\xb7\phantom{\rule{0.166667em}{0ex}}{10}^{-6}$ | −1.27$\phantom{\rule{0.166667em}{0ex}}\xb7\phantom{\rule{0.166667em}{0ex}}{10}^{-4}$ | −52.4 | 2.80 | 0 | −11,500 |

${\lambda}_{111}$ | −2.24$\phantom{\rule{0.166667em}{0ex}}\xb7\phantom{\rule{0.166667em}{0ex}}{10}^{-5}$ | −7.16$\phantom{\rule{0.166667em}{0ex}}\xb7\phantom{\rule{0.166667em}{0ex}}{10}^{-6}$ | −26.2 | −5.35 | −200 | −500 |

${M}_{100}$ | 260,000 | 276,100 | −2.08 | 9.43 | −5000 | 0 |

${M}_{110}$ | 403,234 | 248,314 | 42.8 | −2.50 | 0 | −10,000 |

${M}_{111}$ | 10,621 | 483,372 | 8.86 | 37.9 | 0 | 0 |

**Table A2.**Summary of the elastic constants of Ni gathered from [32]. * Omitted values due to high deviation.

Reference | ${\mathit{C}}_{11}$ (${10}^{11}$Pa) | ${\mathit{C}}_{12}$ (${10}^{11}$Pa) | ${\mathit{C}}_{44}$ (${10}^{11}$Pa) |
---|---|---|---|

Honda et al. | 2.52 | 1.51 | 1.04 |

Bozorth1 et al. | 2.5 | 1.6 | 1.19 |

Bozorth2 et al. Saturated | 2.52 | 1.57 | 1.23 |

Neighbours et al. | 2.53 | 1.52 | 1.24 |

Yamamoto et al. | 2.44 | 1.58 | 1.02 |

Levy et al. | 2.47 | 1.52 | 1.21 |

DeKlerk et al. Saturated | 2.46 | 1.47 | 1.24 |

Shirakawa et al. | 2.55 | 1.69 | 0.90 * |

DeKlerk2 et al. Saturated | 2.46 | 1.48 | 1.22 |

Alers et al. | 2.51 | 1.5 | 1.24 |

Sakurai et al. | 2.51 | 1.53 | 1.24 |

Epstein et al. Saturated | 2.5 | 1.54 | 1.24 |

Vintaikin et al. | 2.47 | 1.44 | 1.24 |

Salama et al. | 2.52 | 1.54 | 1.22 |

Shirakawa2 et al. | 2.88 | 1.81 | 1.24 |

Average | 2.52 | 1.55 | 1.2 |

## Appendix B

## Appendix C

**Figure A2.**Convergence curves for the solution of the presented model with ${t}_{Ni}=$100 nm: (

**a**) magnetic potential, (

**b**) displacement field.

## Appendix D

**Figure A3.**Relative eigenfrequency change $f/{f}_{sat}$ of the three principal axes (

**a**) (100), (

**b**) (110) and (

**c**) (111) for Nickel layer thicknesses ${t}_{Ni}$ in the range of 50–1000 nm derived from the Euler–Bernoulli theory.

## References

- Wang, Y.; Gray, D.; Berry, D.; Gao, J.; Li, M.; Li, J.; Viehland, D. An Extremely Low Equivalent Magnetic Noise Magnetoelectric Sensor. Adv. Mater.
**2011**, 23, 4111–4114. [Google Scholar] [CrossRef] [PubMed] - Gun Lee, D.; Man Kim, S.; Kyung Yoo, Y.; Hyun Han, J.; Won Chun, D.; Kim, Y.C.; Kim, J.; Seon Hwang, K.; Song Kim, T.; Woo Jo, W.; et al. Ultra-sensitive magnetoelectric microcantilever at a low frequency. Appl. Phys. Lett.
**2012**, 101, 182902. [Google Scholar] [CrossRef] - Piorra, A.; Jahns, R.; Teliban, I.; Gugat, J.L.; Gerken, M.; Knöchel, R.; Quandt, E. Magnetoelectric thin film composites with interdigital electrodes. Appl. Phys. Lett.
**2013**, 103, 032902. [Google Scholar] [CrossRef] - Zhai, J.; Xing, Z.; Dong, S.; Li, J.; Viehland, D. Detection of pico-Tesla magnetic fields using magneto-electric sensors at room temperature. Appl. Phys. Lett.
**2006**, 88, 062510. [Google Scholar] [CrossRef] [Green Version] - Schmelz, M.; Stolz, R.; Zakosarenko, V.; Schönau, T.; Anders, S.; Fritzsch, L.; Mück, M.; Meyer, H.G. Field-stable SQUID magnetometer with sub-fT/Hz
^{1/2}-resolution based on sub-micrometer cross-type Josephson tunnel junctions. Supercond. Sci. Technol.**2011**, 24, 065009. [Google Scholar] [CrossRef] - Su, J.; Niekiel, F.; Fichtner, S.; Kirchhof, C.; Meyners, D.; Quandt, E.; Wagner, B.; Lofink, F. Frequency tunable resonant magnetoelectric sensors for the detection of weak magnetic field. J. Micromech. Microeng.
**2020**, 30, 075009. [Google Scholar] [CrossRef] - Fetisov, L.Y.; Serov, V.N.; Chashin, D.V.; Makovkin, S.A.; Srinivasan, G.; Viehland, D.; Fetisov, Y.K. A magnetoelectric sensor of threshold DC magnetic fields. J. Appl. Phys.
**2017**, 121, 154503. [Google Scholar] [CrossRef] - PourhosseiniAsl, M.J.; Chu, Z.; Gao, X.; Dong, S. A hexagonal-framed magnetoelectric composite for magnetic vector measurement. Appl. Phys. Lett.
**2018**, 113, 092902. [Google Scholar] [CrossRef] - Zhang, J.; Li, P.; Wen, Y.; He, W.; Yang, A.; Lu, C. Packaged current-sensing device with self-biased magnetoelectric laminate for low-frequency weak-current detection. Smart Mater. Struct.
**2014**, 23, 095028. [Google Scholar] [CrossRef] - Filippov, D.; Firsova, T.; Laletin, V.; Poddubnaya, N. The magnetoelectric effect in Nickel–GaAs–Nickel structures. Tech. Phys. Lett.
**2017**, 43, 313–315. [Google Scholar] [CrossRef] - Spetzler, B.; Kirchhof, C.; Quandt, E.; McCord, J.; Faupel, F. Magnetic Sensitivity of Bending-Mode Delta-E-Effect Sensors. Phys. Rev. Appl.
**2019**, 12, 064036. [Google Scholar] [CrossRef] - Hui, Y.; Nan, T.; Sun, N.X.; Rinaldi, M. High Resolution Magnetometer Based on a High Frequency Magnetoelectric MEMS-CMOS Oscillator. J. Microelectromech. Syst.
**2015**, 24, 134–143. [Google Scholar] [CrossRef] - Kiser, J.; Finkel, P.; Gao, J.; Dolabdjian, C.; Li, J.; Viehland, D. Stress reconfigurable tunable magnetoelectric resonators as magnetic sensors. Appl. Phys. Lett.
**2013**, 102, 042909. [Google Scholar] [CrossRef] [Green Version] - Shen, Y.; Gao, J.; Wang, Y.; Li, J.; Viehland, D. High non-linear magnetoelectric coefficient in Metglas/PMN-PT laminate composites under zero direct current magnetic bias. J. Appl. Phys.
**2014**, 115, 094102. [Google Scholar] [CrossRef] [Green Version] - Mandal, S.K.; Sreenivasulu, G.; Petrov, V.M.; Srinivasan, G. Magnetization-graded multiferroic composite and magnetoelectric effects at zero bias. Phys. Rev. B
**2011**, 84, 014432. [Google Scholar] [CrossRef] - Bichurin, M.I.; Petrov, R.V.; Leontiev, V.S.; Sokolov, O.V.; Turutin, A.V.; Kuts, V.V.; Kubasov, I.V.; Kislyuk, A.M.; Temirov, A.A.; Malinkovich, M.D.; et al. Self-Biased Bidomain LiNbO3/Ni/Metglas Magnetoelectric Current Sensor. Sensors
**2020**, 20, 7142. [Google Scholar] [CrossRef] - Nguyen, T.; Fleming, Y.; Bender, P.; Grysan, P.; Valle, N.; El Adib, B.; Adjeroud, N.; Arl, D.; Emo, M.; Ghanbaja, J.; et al. Low-Temperature Growth of AlN Films on Magnetostrictive Foils for High-Magnetoelectric-Response Thin-Film Composites. ACS Appl. Mater. Interfaces
**2021**, 13, 30874–30884. [Google Scholar] [CrossRef] - Gojdka, B.; Jahns, R.; Meurisch, K.; Greve, H.; Adelung, R.; Quandt, E.; Knöchel, R.; Faupel, F. Fully integrable magnetic field sensor based on delta-E effect. Appl. Phys. Lett.
**2011**, 99, 223502. [Google Scholar] [CrossRef] [Green Version] - Kim, H.J.; Wang, S.; Xu, C.; Laughlin, D.; Zhu, J.; Piazza, G. Piezoelectric/magnetostrictive MEMS resonant sensor array for in-plane multi-axis magnetic field detection. In Proceedings of the 2017 IEEE 30th International Conference on Micro Electro Mechanical Systems (MEMS), Las Vegas, NV, USA, 22–26 January 2017; pp. 109–112. [Google Scholar] [CrossRef]
- Zhang, Z.; Wu, H.; Sang, L.; Takahashi, Y.; Huang, J.; Wang, L.; Toda, M.; Akita, I.M.; Koide, Y.; Koizumi, S.; et al. Enhancing Delta E Effect at High Temperatures of Galfenol/Ti/Single-Crystal Diamond Resonators for Magnetic Sensing. ACS Appl. Mater. Interfaces
**2020**, 12, 23155–23164. [Google Scholar] [CrossRef] - Giallonardo, J.; Erba, U.; Austa, K.; Palumbo, G. The influence of grain size and texture on the Young’s modulus of nanocrystalline Nickel and Nickel-iron alloys. Philos. Mag.
**2011**, 91, 4594–4605. [Google Scholar] [CrossRef] - Ishizaki, T.; Yatsugi, K.; Akedo, K. Effect of Particle Size on the Magnetic Properties of Ni Nanoparticles Synthesized with Trioctylphosphine as the Capping Agent. Nanomaterials
**2016**, 6, 172. [Google Scholar] [CrossRef] - Hähnlein, B.; Schaaf, P.; Pezoldt, J. Size effect of Young’s modulus in AlN thin layers. J. Appl. Phys.
**2014**, 116, 124306. [Google Scholar] [CrossRef] - Hähnlein, B.; Kovac, J., Jr.; Pezoldt, J. Size effect of the silicon carbide Young’s modulus. Phys. Status Solidi A
**2017**, 214, 1600390. [Google Scholar] [CrossRef] - Krey, M.; Hähnlein, B.; Tonisch, K.; Krischok, S.; Töpfer, H. Automated Parameter Extraction Of ScAlN MEMS Devices Using An Extended Euler-Bernoulli Beam Theory. Sensors
**2020**, 20, 1001. [Google Scholar] [CrossRef] [Green Version] - Haehnlein, B.; Kellner, M.; Krey, M.; Nikpourian, A.; Pezoldt, J.; Michael, S.; Toepfer, H.; Krischok, S.; Tonisch, K. The Angle Dependent Δe Effect in Tin/Aln/Ni Micro Cantilevers. Available online: https://ssrn.com/abstract=4112978 (accessed on 18 May 2022).
- Cullity, B.D.; Graham, C.D. Introduction to Magnetic Materials; John Wiley & Sons: Hoboken, NJ, USA, 2008; pp. 197–273. [Google Scholar] [CrossRef]
- Carr, W. Invar and volume magnetostriction. J. Magn. Magn. Mater.
**1979**, 10, 197–204. [Google Scholar] [CrossRef] - Masiyama, Y. On the magnetostriction of a single crystal of Nickel. Sci. Rep. Tohoku Imp. Univ.
**1928**, 17, 945–961. [Google Scholar] - Spetzler, B.; Golubeva, E.V.; Müller, C.; McCord, J.; Faupel, F. Frequency Dependency of the Delta-E Effect and the Sensitivity of Delta-E Effect Magnetic Field Sensors. Sensors
**2019**, 19, 4769. [Google Scholar] [CrossRef] [Green Version] - Rösler, J.; Harders, H.; Bäker, M. Mechanisches Verhalten der Werkstoffe; Vieweg+Teubner: Wiesbaden, Germany, 2019; pp. 51–53. [Google Scholar] [CrossRef]
- Ledbetter, H.; Reed, R. Elastic Properties of Metals and Alloys, I. Iron, Nickel, and Iron-Nickel Alloys. J. Phys. Chem. Ref. Data
**1973**, 2, 531–617. [Google Scholar] [CrossRef] [Green Version] - Yamamoto, M. The Elastic Constants of Nickel Single Crystals. J. Jpn. I. Met. Mater.
**1942**, 6, 331–338. [Google Scholar] [CrossRef] - McCarthy, E.; Bellew, A.; Sader, J.; Boland, J. Poisson’s ratio of individual metal nanowires. Nat. Commun.
**2014**, 5, 4336. [Google Scholar] [CrossRef] [Green Version] - Zhou, H.; Pei, Y.; Fang, D. Magnetic Field Tunable Small-scale Mechanical Properties of Nickel Single Crystals Measured by Nanoindentation Technique. Sci. Rep.
**2014**, 4, 4583. [Google Scholar] [CrossRef] [PubMed] - Baxy, A.; Sarkar, A. Natural frequencies of a rotating curved cantilever beam: A perturbation method-based approach. Proc. Inst. Mech. Eng. Part C J. Mech. Eng. Sci.
**2020**, 234, 1706–1719. [Google Scholar] [CrossRef] - Greve, H.; Woltermann, E.; Quenzer, H.J.; Wagner, B.; Quandt, E. Giant magnetoelectric coefficients in (Fe90Co10)78Si12B10-AlN thin film composites. Appl. Phys. Lett.
**2010**, 96, 182501. [Google Scholar] [CrossRef] - Lou, J.; Insignares, R.E.; Cai, Z.; Ziemer, K.S.; Liu, M.; Sun, N.X. Soft magnetism, magnetostriction, and microwave properties of FeGaB thin films. Appl. Phys. Lett.
**2007**, 91, 182504. [Google Scholar] [CrossRef] - Yang, P.; Peng, S.; Wu, X.B.; Wan, J.G.; Zhu, J.S. Magnetoelectric study in Terfenol-D/PFNT laminate composite. Integr. Ferroelectr.
**2008**, 99, 86–92. [Google Scholar] [CrossRef] - Nan, T.; Hui, Y.; Rinaldi, M.; Sun, N.X. Self-Biased 215 MHz Magnetoelectric NEMS Resonator for Ultra-Sensitive DC Magnetic Field Detection. Sci. Rep.
**2013**, 3, 1985. [Google Scholar] [CrossRef] [Green Version] - Kirchner, H. Über den Einfluß von Zug, Druck und Torsion auf die Längsmagnetostriktion. Ann. Phys.
**1936**, 419, 49–69. [Google Scholar] [CrossRef] - Ludwig, A.; Quandt, E. Optimization of the Delta-E effect in thin films and multilayers by magnetic field annealing. IEEE Trans. Magn.
**2002**, 38, 2829–2831. [Google Scholar] [CrossRef] - Coey, J.M. Magnetism and Magnetic Materials; Cambridge University Press: Cambridge, UK, 2010; pp. 264–304. [Google Scholar] [CrossRef] [Green Version]
- Ciria, M.; Arnaudas, J.I.; Benito, L.; de la Fuente, C.; del Moral, A.; Ha, J.K.; O’Handley, R.C. Magnetoelastic coupling in thin films with weak out-of-plane anisotropy. Phys. Rev. B
**2003**, 67, 024429. [Google Scholar] [CrossRef] - Liang, X.; Dong, C.; Chen, H.; Wang, J.; Wei, Y.; Zaeimbashi, M.; He, Y.; Matyushov, A.; Sun, C.; Sun, N. A Review of Thin-Film Magnetoelastic Materials for Magnetoelectric Applications. Sensors
**2020**, 20, 1532. [Google Scholar] [CrossRef] [Green Version] - Spetzler, B.; Golubeva, E.V.; Friedrich, R.M.; Zabel, S.; Kirchhof, C.; Meyners, D.; McCord, J.; Faupel, F. Magnetoelastic Coupling and Delta-E Effect in Magnetoelectric Torsion Mode Resonators. Sensors
**2021**, 21, 2022. [Google Scholar] [CrossRef] - Durdaut, P.; Rubiola, E.; Friedt, J.M.; Müller, C.; Spetzler, B.; Kirchhof, C.; Meyners, D.; Quandt, E.; Faupel, F.; McCord, J.; et al. Fundamental Noise Limits and Sensitivity of Piezoelectrically Driven Magnetoelastic Cantilevers. J. Microelectromechanical Syst.
**2020**, 29, 1347–1361. [Google Scholar] [CrossRef] - Li, M.; Matyushov, A.; Dong, C.; Chen, H.; Lin, H.; Nan, T.; Qian, Z.; Rinaldi, M.; Lin, Y.; Sun, N.X. Ultra-sensitive NEMS magnetoelectric sensor for picotesla DC magnetic field detection. Appl. Phys. Lett.
**2017**, 110, 143510. [Google Scholar] [CrossRef] - Linzen, S.; Schmidt, F.; Schmidl, F.; Mans, M.; Hesse, O.; Nitsche, F.; Kaiser, G.; Müller, S.; Seidel, P. A thin film HTSC-Hall magnetometer - development and application. Phys. C Supercond.
**2002**, 372–376, 146–149. [Google Scholar] [CrossRef] - Webster, W.L. Magnetostriction and change of resistance in single crystals of iron and Nickel. Proc. Phys. Soc.
**1930**, 42, 431–440. [Google Scholar] [CrossRef] - Daniel, L. An analytical model for the magnetostriction strain of ferromagnetic materials subjected to multiaxial stress. Eur. Phys. J. Appl. Phys.
**2018**, 83, 30904. [Google Scholar] [CrossRef] [Green Version] - Namazu, T.; Inoue, S.; Takemoto, H.; Koterazawa, K. Mechanical Properties of Polycrystalline Titanium Nitride Films Measured by XRD Tensile Testing. IEEJ Trans. Sens. Micromachines
**2005**, 125, 374–379. [Google Scholar] [CrossRef] [Green Version]

**Figure 1.**(

**a**) SEM images of 4 $\mathsf{\mu}$$\mathrm{m}$ wide magnetoelectric cantilevers consisting of a TiN( 90 $\mathrm{n}$$\mathrm{m}$)/ AlN( 450 $\mathrm{n}$$\mathrm{m}$)/Ni( 100 $\mathrm{n}$$\mathrm{m}$) layer stack investigated in recent work [26]. (

**b**) Eigenfrequency characteristics in dependency of the magnetic flux of four 25 $\mathsf{\mu}$$\mathrm{m}$ long and identically aligned cantilevers as marked in (

**a**). (

**c**) Solution of the 2D model used for the simulation study with the layer configuration from (

**a**). The bending effect due to magnetostrictive strains in the 25 $\mathsf{\mu}$$\mathrm{m}$ cantilever is upscaled for better visibility.

**Figure 2.**(

**a**) Computed magnetic-field-dependent curves of Young’s modulus for the three principal axes. (

**b**) Eigenfrequencies of the simulated cantilevers in magnetic saturation as a function of the crystalline orientation of the Nickel layer and its thickness.

**Figure 3.**(

**a**) Deflection in magnetic saturation of the simulated cantilever for different thicknesses ${t}_{Ni}$. (

**b**) Influence of the cantilever curvature on the eigenfrequency. The curvature caused by magnetostriction is derived for comparison from (

**a**).

**Figure 4.**Relative eigenfrequency change $f/{f}_{sat}$ (left hand side) and the respective specific sensitivity $\partial f/\partial B$ (right hand side) of the three principal axes (

**a**) (100), (

**b**) (110) and (

**c**) (111) for Nickel layer thicknesses ${t}_{Ni}$ in the range of 50–1000 nm. The point of highest absolute sensitivity as well as the dynamic range is marked by the lines, respectively.

**Figure 5.**(

**a**) Absolute values of the maximum sensitivities derived from Figure 4 (FEM) and from the Euler–Bernoulli theory (EBT) for the three principal axes and ${t}_{Ni,sat}$ at the given offsets of the magnetic flux. The experimentally achieved sensitivity is added for comparison. The value for zero thickness is extrapolated. (

**b**) Extracted dynamic range in dependence of $|{S}_{H}|$ for the three orientations.

**Table 1.**Comparison of simulated and experimental sensitivities of the natural frequency of electromechanical system based on magnetoelectric sensors. (Values calculated according to Equation (10) if not given in the reference). * Sensitivity for the second eigenmode.

Material | Reference | Sensitivity (1/T) |
---|---|---|

Ni(100)/AlN/TiN${}^{sim}$ | this work | −14.9 |

Ni(110)/AlN/TiN${}^{sim}$ | this work | −41.3 |

Ni(111)/AlN/TiN${}^{sim}$ | this work | 8.8 |

poly-Ni/AlN/TiN${}^{exp}$ | [26] | −0.9 …−1.4 |

FeCoSiB/poly-Si/AlN${}^{exp}$ | [11] | 10 |

FeCoSiB/poly-Si/AlN${}^{exp}$ | [11] | 13 * |

FeCoSiB/poly-Si/AlN${}^{sim}$ | [11] | 48 * |

FeCoB/Al/AlN/Pt${}^{exp}$ | [19] | −0.7 |

FeGaB/AlN/Pt${}^{exp}$ | [48] | −2.2 |

FeGa/Ti/Diamond${}^{exp}$ | [20] | 0.5 |

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Hähnlein, B.; Sagar, N.; Honig, H.; Krischok, S.; Tonisch, K.
Anisotropy of the ΔE Effect in Ni-Based Magnetoelectric Cantilevers: A Finite Element Method Analysis. *Sensors* **2022**, *22*, 4958.
https://doi.org/10.3390/s22134958

**AMA Style**

Hähnlein B, Sagar N, Honig H, Krischok S, Tonisch K.
Anisotropy of the ΔE Effect in Ni-Based Magnetoelectric Cantilevers: A Finite Element Method Analysis. *Sensors*. 2022; 22(13):4958.
https://doi.org/10.3390/s22134958

**Chicago/Turabian Style**

Hähnlein, Bernd, Neha Sagar, Hauke Honig, Stefan Krischok, and Katja Tonisch.
2022. "Anisotropy of the ΔE Effect in Ni-Based Magnetoelectric Cantilevers: A Finite Element Method Analysis" *Sensors* 22, no. 13: 4958.
https://doi.org/10.3390/s22134958